Minhao Pu*, Luisa Ottaviano, Elizaveta Semenova, and Kresten Yvind**
DTU Fotonik, Department of Photonics Engineering, Technical University of Denmark, Building 343, DK-2800 Lyngby, Denmark
The combination of nonlinear and integrated photonics has recently seen a surge with Kerr frequency comb
generation in micro-resonators1 as the most significant achievement. Efficient nonlinear photonic chips have
myriad applications including high speed optical signal processing2,3, on-chip multi-wavelength lasers4,5,
(AlGaAs) exhibits very high material nonlinearity and low nonlinear loss9,10 when operated below half its
bandgap energy. However, difficulties in device processing and low device effective nonlinearity made Kerr frequency comb generation elusive. Here, we demonstrate AlGaAs-on-insulator as a nonlinear platform at telecom wavelengths. Using newly developed fabrication processes, we show high-quality-factor (Q>105)
micro-resonators with integrated bus waveguides in a planar circuit where optical parametric oscillation is achieved with a record low threshold power of 3 mW and a frequency comb spanning 350 nm is obtained.
Our demonstration shows the huge potential of the AlGaAs-on-insulator platform in integrated nonlinear photonics.
Desirable material properties for all-optical χ(3) nonlinear chips are a high Kerr nonlinearity and low linear and nonlinear losses to enable high four-wave mixing (FWM) efficiency and parametric gain. Many material platforms have been investigated showing the different trade-offs between nonlinearity and losses2-5,11-16. In addition to good intrinsic material properties, the ability to perform accurate and high yield processing is desirable in order to integrate additional functionalities on the same chip and also to decrease linear losses. Silicon-on-insulator is the model system for integration2. It supports a large index contrast and shallow etch depths, enabling patterning sub-
micron structures with smooth sidewalls. However, due to two-photon absorption (TPA) at telecom wavelengths,
e.g. 1550 nm, high parametric gain15 and Kerr frequency comb generation16 have only been achieved by pumping at
wavelengths beyond 2000 nm.
Aluminium gallium arsenide (AlxGa1-xAs) was early identified as a promising candidate and even nominated as the “silicon of nonlinear optics”9 when operated just below half its bandgap energy. It offers a high refractive index
17-19 -17 2 (n≈3.3) and a nonlinear index (n2) on the order of 10 W/m , a large transparency window (from near- to mid- infrared), and the ability to engineer the material bandgap by varying the alloy composition (x)19. Its bandgap can be tailored in such a way that TPA, which is the main detrimental effect for the FWM process, is mitigated and at the same time, the three-photon absorption is low10 while a high material nonlinearity is maintained. Over the past two
decades, efforts have been made to realize efficient nonlinear processes in AlGaAs waveguides17-19. However, the
fabrication of such waveguides with very high and narrow mesa structures becomes very challenging and prevents
advanced designs that go beyond simple straight waveguides. In addition, the low vertical index contrast of such
waveguides limits the effective nonlinearity.
To enhance light confinement and relax the etching process requirements, we propose an AlGaAs-on-insulator
(AlGaAsOI) platform as shown in Fig. 1a. In this layout, a thin AlxGa1-xAs layer on top of a low index insulator
layer resides on a semiconductor substrate. Wafer bonding and substrate removal are used to realize the structure. In this letter, the aluminium fraction (x) is 17%, which makes the material bandgap 1.63 eV and the refractive index
3.33. Thanks to the large index contrast (~55%) of this layout, light can be confined in a sub-micron waveguide
2 core. As the nonlinear parameter (γ) is highly dependent on the waveguide effective mode area (Aeff) as expressed
-1 -1 by γ=2πn2/λAeff, an ultra-high effective nonlinearity of about 660 W m , which is orders of magnitude higher than
5 that of a typical Si3N4 waveguide , can be obtained for an AlGaAsOI waveguide using a cross-section dimension of
320 nm×630 nm (see Methods). In addition, the waveguide dispersion dominates over material dispersion for sub- wavelength sized waveguides and therefore the group velocity dispersion (GVD) can be engineered from the normal dispersion of bulk material to anomalous dispersion (Fig. 1b), which is required to achieve parametric gain in nonlinear processes15. High index-contrast waveguide device performance is typically limited by linear loss induced
by light scattering from surface roughness16. High quality epitaxial material growth and substrate removal is required to ensure smoothness for top and bottom waveguide surfaces while good lithography and dry etching processes define the waveguide sidewall surface roughness. A critical element is the choice of etch stop layer in the substrate removal process (see Methods) as e.g. hydrofluoric acid etching of Al(Ga)As leaves a too rough surface20.
Fig. 1c shows a scanning electron microscope (SEM) picture of a fabricated AlGaAsOI waveguide with about
1.4 dB/cm linear loss. Combining the ultra-high effective nonlinearity and low loss, AlGaAsOI can be used for ultra-
efficient nonlinear parametric processes such as low-threshold Kerr frequency comb generation once a high quality factor (Q) micro-resonator is realized.
Fig. 2a shows a SEM picture of an 810-μm long race-track-shaped AlGaAsOI micro-resonator. Fig. 2b shows a coupling gap of 170 nm for the resonator where the light propagating in the 450 nm-wide bus waveguide can be evanescently coupled to the 630 nm-wide curved (17.5 μm radius) waveguide of the resonator. The resonator works in the under-coupled regime and its transmission is shown in Fig. 2c for the transverse electric (TE) mode. Only one mode family with a free spectral range (FSR) of ~0.82 nm (98 GHz) is observed in the spectrum, which implies that the resonator waveguide with anomalous dispersion can be operated in a single-mode state. Therefore, the dispersion distortion induced by inter-mode interaction between different mode families can be completely avoided, which is preferable for Kerr frequency comb generation (especially temporal soliton formation) but not attainable in all nonlinear material platforms21. Fig. 2d shows the measured transmission spectrum for the resonance at 1589.64 nm and the measured linewidth is around 9.6 pm which corresponds to a Q of ~165,600. The measured Q for all the
devices ranges from 1.5×105 to 2.0×105, which is more than an order of magnitude higher than previously demonstrated Q for AlGaAs micro-ring resonators22.
Kerr frequency comb generation is based on optical parametric oscillation (OPO), which relies on a
combination of parametric amplification and oscillation as a result of the nonlinear FWM processes within the
micro-resonator. As a continuous wave pump light is tuned into a cavity resonance to achieve thermal soft-locking23, the built-up intra-cavity power triggers OPO at a critical power threshold when the round-trip parametric gain exceeds the round-trip loss of the resonator. To satisfy the momentum conservation in the FWM process, the pump energy can only be transferred to equispaced frequencies within the supported resonances of the micro-resonator1
and thus form a frequency comb at output as illustrated in Fig. 3a. The measured spectrum of an AlGaAsOI micro-
resonator is shown in Fig. 3b when a pump power of 72 mW was coupled into the bus waveguide. A frequency
comb with the native line spacing (single FSR) spanning over about 350 nm was observed.
The threshold power in the bus waveguide can be estimated by the expression24 1.54( ) 2 2 2 2, 𝜋𝜋 𝑄𝑄𝐶𝐶 𝑛𝑛 𝐿𝐿𝐴𝐴𝑒𝑒𝑒𝑒𝑒𝑒 1 𝑡𝑡ℎ 2 𝑃𝑃 𝑃𝑃 ≈ 𝑄𝑄𝐿𝐿 𝑛𝑛 𝜆𝜆 ∙ 𝑄𝑄𝐿𝐿 where L and λp, are the cavity length and pump wavelength, and QC and QL are the coupling and loaded quality factors of the resonator, respectively. As QL and L are correlated, we measured the threshold power for micro- resonators with different cavity lengths (FSR ranging from 98 GHz to 995 GHz) to find their influences on threshold
power. The obtained minimum threshold power was 3 mW for a ring-shaped micro-resonator (see inset of Fig. 4a)
5 operated in the under-coupling condition with a QL of about 10 . The output power of the primary OPO sideband increases significantly at threshold, as shown in Fig. 4a. Fig. 4b shows the measured output spectrum for this resonator with a pump power (4.5 mW) slightly above the threshold. It shows a typical OPO initial state in which widely spaced (multi-FSR
25 spacing) primary sidebands are generated . The measured threshold power for different devices as a function of QL is shown in Fig. 4c, where most of micro-resonators are seen to have milliwatt-level thresholds, although micro-resonators
with smaller FSR exhibit slightly higher threshold. The measured data follows the theoretically predicted threshold trend as shown by the coloured bands, and a sub-mW threshold power can be expected with further improvement of resonator design26 and fabrication processes.
As the dynamics of Kerr frequency comb generation have been extensively studied23-25 and mode-locked
combs have been demonstrated21,27, Kerr frequency comb technologies are approaching practical applications.
Planar integration platforms are critical for practical systems because of their robustness and potential for a fully integrated comb system with on-chip light sources. Low threshold is crucial for the realization of such a system.
Table 1 summarizes several planar integrated nonlinear material platforms where a frequency comb has been
4 5 11 12 demonstrated at telecom wavelengths, including Hydex , Si3N4 , AlN , Diamond and AlGaAs. The linear
refractive index of AlGaAs is the highest among these platforms, which makes it the most suitable platform for
compact circuits. In addition, the material nonlinear index of AlGaAs is orders of magnitude larger than those of the
other platforms. These intrinsic material properties make AlGaAsOI an ultra-efficient platform for nonlinear
parametric processes. Therefore, even though the QL of our device is relatively low, the OPO threshold power for the
AlGaAsOI platform is the lowest compared with the other platforms. In line with the fast-growing hybrid integration trend to combine different materials in multiple levels on a single CMOS compatible chip, the AlGaAsOI platform is
very promising for realizing a fully-integrated comb system.
Because of the wide transparency window of AlGaAs materials, the frequency comb can potentially be
extended into the mid-infrared with proper dispersion engineering. Besides comb generation, we have recently
demonstrated wavelength conversion of a serial data signal at a record high speed (beyond terabaud) in this
platform28. An ultra-broad bandwidth and ultra-high efficiency make AlGaAsOI an excellent platform for optical signal processing in telecommunications. Moreover, AlGaAs exhibits strong χ(2) effects29 due to its non-
centrosymmetric crystal structure. Therefore, the AlGaAsOI platform is also suitable for combining both χ(2) and χ(3)
effects to obtain, for example, multi-octave spanning combs30.
Device fabrication. The preparation of AlGaAsOI samples includes wafer growth, wafer bonding, and substrate removal. A 320-nm thick layer of Al0.17Ga0.83As was grown in a low-pressure metalorganic vapour phase epitaxy
(MOVPE) reactor on a 50-mm GaAs (100) substrate with sacrificial layers. After depositing a 3-μm thick silica layer on the AlGaAs layer using plasma-enhanced chemical vapour deposition (PECVD), a 90-nm thick
Benzocyclobutene (BCB) layer was used as a bonding polymer between the grown wafer and another 50-mm semiconductor substrate covered with a 10-nm thick silica layer. The bonding process was performed under partial vacuum (~3×10-2 Pa) at 250 ⁰C for one hour in a wafer bonding system, while a force of 750 N was applied to the wafers. Subsequently, the GaAs substrate and the sacrificial layers were removed by wet etching. It is crucial to use proper etch stop layer and etchant as the etching by-products may result in roughness and absorption sites on the
AlGaAs film surface (Supplementary Fig. 1). Electron beam lithography (EBL, JEOL JBX-9500FS) was used to define the device pattern in the electron beam resist hydrogen silsesquioxane (HSQ, Dow Corning FOX-15). To get a smooth pattern definition for bent waveguides in micro-resonators, a multi-pass exposure was applied to mitigate the stitching between pattern segments fractured during the EBL (Supplementary Fig. 2). The device pattern was then transferred into the AlGaAs layer using a boron trichloride (BCl3)-based dry etching process in an inductive coupled plasma reactive ion etching (ICP-RIE) machine. As the refractive index of HSQ is relatively low (similar to
SiO2), it was kept on top of the AlGaAs device pattern. Finally, clad in a 3-μm thick silica layer using PECVD, the chip was cleaved to form the input and output facets where nano-tapers enabled efficient chip-to-fibre coupling for characterization.
Modelling. Waveguide dispersion was calculated using a finite-element method mode solver (COMSOL) for the TE mode in the wavelength range between 1300 nm and 1800 nm. The Sellmeier equation was used to incorporate the dispersion of SiO2 and the modified single effective oscillator model was used for AlGaAs. The dispersion of HSQ, a leftover electron beam resist on top of AlGaAs, was assumed to be the same as that of SiO2.
Measurement of nonlinearity. A FWM measurement was performed using two continuous wave signals (one for
the pump and one for the signal) in a 3-mm long AlGaAsOI nano-waveguide with a cross-section of
320 nm×630 nm. The pump-to-signal detuning was less than 1 nm to ensure phase matching14. We measured the
dependence of conversion efficiency on pump power (Supplementary Fig. 4) and extracted the nonlinear
coefficient γ by fitting the expression18𝜂𝜂
( ) = = (0) ( ) 𝑃𝑃𝑖𝑖𝑖𝑖𝑖𝑖𝑖𝑖𝑖𝑖 𝐿𝐿 2 𝜂𝜂 �𝛾𝛾𝑃𝑃𝑝𝑝𝑝𝑝𝑝𝑝𝑝𝑝 𝐿𝐿𝑒𝑒𝑒𝑒𝑒𝑒� 𝑃𝑃𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠 𝐿𝐿 where = (1 )/ is the effective waveguide length and α the linear loss coefficient. The conversion −𝛼𝛼𝛼𝛼 𝑒𝑒𝑒𝑒𝑒𝑒 efficiency𝐿𝐿 was determined− 𝑒𝑒 from𝛼𝛼 the spectrum at the chip output. The pump power was estimated by subtracting the
chip-to-fibre coupling loss from the fibre output power. The waveguide propagation loss (1.4 dB/cm) was measured
at 1550 nm using the modified cutback method (Supplementary Fig. 3). Assuming the input and output coupling are
the same, we estimated the coupling loss to be ~2.7 dB/facet by subtracting the waveguide loss from the fibre-to-
fibre insertion loss (~6.3 dB). We obtained an ultra-high nonlinear coefficient: ~660 W-1m-1.
The authors would like to thank Jan W. Thomsen at Copenhagen University, Christophe Peucheret at Université de
Rennes 1, Molly Piels, Hao Hu, Leif K. Oxenløwe and Jesper Mørk at the Technical University of Denmark for motivating and helpful discussions and comments on this manuscript. The authors acknowledge financial support from Villum Fonden via the Centre of Excellence Nanophotonics for terabit optical communication (NATEC). M. P. also acknowledges the Danish Research Council via the SiMOF project (11-117031).
M.P. designed the device. M. P., L.O., and E.S. fabricated the device. M.P. performed the device characterization and
analysed the data. K.Y. conceived the idea and supervised the work. M.P. and K.Y. wrote the manuscript.
1. Kippenberg, T. J., Holzwarth, R. & Diddams, S. A. Microresonator-based optical frequency combs. Science
332 555-559 (2011).
2. Leuthold, J., Koos, C. & Freude, W. Nonlinear silicon photonics. Nature Photon. 4, 535–544 (2010).
3. Eggleton, B. J., Luther-Davies, B. & Richardson, K. Chalcogenide photonics. Nature Photon. 5, 141–148
4. Razzari, L. et al. CMOS-compatible integrated optical hyper-parametric oscillator. Nature Photon. 4 41-45
5. Levy, J. S. et al. CMOS-compatible multiple-wavelength oscillator for on-chip optical interconnects. Nature
Photon. 4 37-40 (2010).
6. Udem, T., Holzwarth, R. & Hänsch, T. W. Optical frequency metrology. Nature 416, 233–237 (2002).
7. Schliesser, A., Picque, N. & Hänsch, T. W. Mid-infrared frequency combs. Nature Photon. 6, 440–449 (2012).
8. Silverstone, J. W. et al. On-chip quantum interference between silicon photon-pair sources. Nature Photon. 8
9. Stegeman, G. I. et al. AlGaAs below half bandgap: the silicon of nonlinear optical materials. Int. J. Nonlinear
Opt. Phys. 3 347-371 (1994).
10. Aitchison, J. S., Hutchings, D. C., Kang, J. U., Stegeman, G. I. & Villeneuve, A. The nonlinear optical
properties of AlGaAs at the half band gap. IEEE J. Quant. Electron. 33 341-348 (1997).
11. Jung, H., Xiong, C., Fong, K. Y., Zhang, X. & Tang, H. X. Optical frequency comb generation from
aluminium nitride microring resonator. Opt. Lett. 38 2810-2812 (2013).
12. Hausmann, B. J. M., Bulu, I., Venkataraman, V., Deotare, P. & Loncar, M. Diamond nonlinear photonics.
Nature Photon. 8, 369–374 (2014).
13. Kuyken, B. et al. Nonlinear properties of and nonlinear processing in hydrogenated amorphous silicon
waveguide. Opt. Express 19 B146-B153 (2011).
14. Dave, U. D. et al. Nonlinear properties of dispersion engineered InGaP photonic wire waveguides in the
telecommunication wavelength range. Opt. Express 23 4650-4657 (2015).
15. Liu, X., Osgood, R. M., Vlasov, Y. A. & Green, W. M. J. Mid-infrared optical parametric amplifier using
silicon nanophotonic waveguides. Nature Photon 4, 557–560 (2010).
16. Griffith, A. G. et al. Silicon-chip mid-infrared frequency comb generation. Nature Commun. 6 6299 (2015).
17. Dolgaleva, K., Ng, W. C., Qian, L. & Aitchison, J. I. Compact highly-nonlinear AlGaAs waveguides for
efficient wavelength conversion. Opt. Express 19 12440-12455 (2011).
18. Lacava, C., Pusino, V., Minzioni, P., Sorel, M. & Cristiani, I. Nonlinear properties of AlGaAs waveguides in
continuous wave operation regime. Opt. Express 22 5291-5298 (2014).
19. Wathen, J. J. et al. Efficient continuous-wave four-wave mixing in bandgap-engineered AlGaAs waveguides.
Opt. Lett. 39 3161-3164 (2014).
20. Cheng, C. et al. Epitaxial lift-off process for gallium arsenide substrate reuse and flexible electronics. Nature
Commun. 4 1577 (2013).
21. Herr, T. et al. Mode spectrum and temporal soliton formation in optical microresonators. Phys. Rev. Lett. 113
22. Kultavewuti, P., Pusino, V., Sorel, M. & Aitchison, J. S. Low-power continuous-wave four-wave mixing
wavelength conversion in AlGaAs-nanowaveguide microresonators. Opt. Lett. 40 3029-3032 (2015).
23. Grudinin, I. S., Yu, N. & Maleki, L. Generation of optical frequency combs with a CaF2 resonator. Opt. Lett.
34, 878-880 (2009).
24. Matsko, A. B., Savchenkov, A. A., Strekalov, D., Ilchenko, V. S. & Maleki, L. Optical hyperparametric
oscillations in a whispering-gallery-mode resonator: threshold and phase diffusion. Phys. Rev. A 71 033804
25. Herr, T. et al. Universal formation dynamics and noise of Kerr-frequency combs in microresonators. Nature
Photon. 6 480-487 (2012).
26. Spencer, D. T., Bauters, J. F., Heck, M. J. R., & Bowers, J. E. Integrated waveguide coupled Si3N4 resonators
in the ultrahigh-Q regime. Optica 1 153-157 (2014).
27. Xue, X. et al. Mode-locked dark pulse Kerr combs in normal-dispersion microresonators. Nature Photon. 9
28. Pu, M. et al. AlGaAs-on-insulator nanowire with 750 nm FWM bandwidth, -9 dB CW conversion efficiency,
and ultrafast operation enabling record Tbaud wavelength conversion. in Optical Fiber Communication
Conference Post Deadline Papers Th5A.3.(2015).
29. Mariani, S. et al. Second harmonic generation in AlGaAs microdisks in the telecom range. Opt. Lett. 39 3062-
30. Jung, H., Stoll, R., Guo, X., Fischer, D. & Tang, H. X. Green, red, and IR frequency comb line generation
from single IR pump in AlN microring resonator. Optica 1 396-399 (2014).
9 a b c SiO2 600 ) -1 nm 0 nm -1 320 AlxGa1‐xAs HSQ -600 630 nm AlGaAs -1200
SiO2 GVD (ps km Waveguide SiO2 Bulk material -1800 200 nm Substrate 1300 1400 1500 1600 1700 1800 Wavelength (nm) Fig. 1 | AlGaAs-on-insulator nano-waveguide. a, Schematic drawing of an AlGaAs-on-insulator
(AlGaAsOI) nano-waveguide with the simulated electric field distribution for the fundamental transverse electric (TE) mode. b, Calculated group velocity dispersion (GVD) versus wavelength for the waveguide with 320 nm×630 nm cross-section dimensions. The dashed curve shows the GVD for bulk AlGaAs material. c, Scanning electron microscope (SEM) picture of an AlGaAsOI nano-waveguide (highlighted in blue) after the dry-etching process. a b Input
20 μm Output
c 0 d 1.0 -3 0.8 -6 0.6 9.6 pm
-9 0.4 Data -12 0.2 Fit
-15 Normalized transmission 0.0 Normalized transmission(dB) 1583 1584 1585 1586 1587 1588 1589 1590 1591 1589.60 1589.64 1589.68 Wavelength (nm) Wavelength (nm) Fig. 2 | AlGaAs-on-insulator microresonator. a, Top-view SEM image of the AlGaAsOI micro-resonator showing ring and bus waveguide. b, Isometric view SEM image of the coupling region of the AlGaAsOI micro-resonator where the AlGaAs material is indicated in blue. c, Measured (normalized) transmission spectrum of the AlGaAsOI micro-resonator. d, Measured (normalized) transmission spectrum around the resonance of the AlGaAsOI micro-resonator at 1590 nm with a loaded quality-factor (Q) of ~165,600. a Degenerate FWM Non‐degenerate FWM
ħω1 ħω2 ħω1 ħω3
P ħω1 ħω3 ħω2 ħω4
f b 0 0 -20 98 GHz -40 -20 -60 1676 1678
-60 1400 1450 1500 1550 1600 1650 1700 1750 1800 Wavelength (nm) Fig. 3 | Optical frequency comb generation in an AlGaAs-on-insulator micro-resonator. a, A single- frequency pump light coupled into a high Q micro-resonator enables efficient parametric processes
(degenerate and non-degenerate four-wave mixing) in the resonator and allows new frequency generation in the supported modes of the micro-resonator. b, The output spectrum of an 810-μm long AlGaAsOI micro-resonator when a 72-mW pump was coupled into the resonator at ~1590 nm. A frequency comb was generated with a line spacing of 98 GHz over a wavelength range of about 350 nm. ab0 c 98 GHz -20 102 730 GHz W)
m 995 GHz
-20 ( 101
25 μm -40 power
ld 0 Power (dBm) Power 3 mW o 10 Power (dBm) h -60
-60 res -1
Th 10 110 1450 1500 1550 1600 1650 1700 105 106 Pump power (mW) Wavelength (nm) Loaded quality factor Fig. 4 | Optical parametric oscillation threshold measurement. a, Measured primary sideband power at the chip output as a function of pump power in the bus waveguide for a 25-μm diameter under-coupled micro-resonator with a FSR of 995 GHz as shown in the inset. A significant power increase was observed at the threshold of 3.1 mW. b, The output spectrum of optical parametric oscillation when the pump power was increased to just above the threshold power (4.5 mW) for the same micro-resonator in a. c, The measured threshold power for micro-resonators with three different FSRs: 98 GHz (red), 730 GHz (green), and 995 GHz (blue). The coloured bands shows the theoretical threshold power ranges for the different micro-resonators (from critical-coupling with QC=2QL to under-coupling with QC=10QL).
Table 1 Comparison of planar nonlinear platforms for frequency comb generation at telecom wavelengths Material n n2 Height Width Comb line QL Pth Platform (W/m2) (μm) (μm) spacing (GHz) (mW) Hydex4 1.7 1.2×10-19 1.45 1.50 200 1×106 50 5 -19 * 5 Si3N4 2.0 2.5×10 0.71 1.70 580 2×10 50 AlN11 2.1 2.3×10-19 0.65 3.50 435 8×105 200 Diamond12 2.4 8.2×10-20 0.95 0.85 925 1×106 20 -17 5 Al0.17Ga0.83As 3.3 2.6×10 0.32 0.62 995 1×10 3 (this work) *Taken as a base width with 20° sidewall angle.
Supplementary information for
AlGaAs-on-Insulator Nonlinear Photonics
Minhao Pu*, Luisa Ottaviano, Elizaveta Semenova, and Kresten Yvind**
DTU Fotonik, Department of Photonics Engineering, Technical University of Denmark, Building 343, DK-2800 Lyngby, Denmark
a b 300 nm 300 nm
Fig. 1 | Device surface roughness comparison. Scanning electron microscope (SEM) pictures of etched patterns on AlGaAs-on-insulator (AlGaAsOI) wafers fabricated by using different substrate removal processes: a, Large roughnesses are observed at the top and bottom surfaces of the AlGaAs film when a conventional etch stop layer1 is used. b, Significant improvement concerning surface smoothness can be observed when a proper etch stop layer was used2. AlGaAs material is denoted by the artificial blue colour in both pictures. Etch mask hydrogen silsesquioxane (HSQ) is left on top of AlGaAs patterns. The same dry etching processes are used in both cases. a b
500 nm 500 nm
Fig. 2 | Electron beam lithography (EBL) patterning comparison. SEM pictures of developed curved pattern in e-beam resist HSQ with different EBL processes: a, Standard EBL process results in severe stitching (denoted by arrows) between fractured pattern segments. The stitching effect may be due to resist charging in EBL process3. b, The multi-pass EBL process mitigates the stitching effect and enables smooth curved waveguide patterning.
a b c 8.5 8.0 y=1.36x+5.47 HSQ 7.5
7.0 HSQ Cladding AlGaAs PECVD SiO2 AlGaAs 6.5 Taper tip
Cladding 6.0 Insertion(dB) loss 500 nm PECVD SiO2 5.5 BCB 100 nm 0.6 0.9 1.2 1.5 1.8 Semiconductor substrate Length (cm)
Fig. 3 | Fabricated AlGaAsOI waveguide device and its loss measurment. a, SEM cross-section picture of an AlGaAsOI nano-waveguide (denoted by the artificial blue colour) cladded in SiO2. Benzocyclobutene
(BCB) was used as bonding layer as denoted by the yellow colour. A strong light confinement can be achieved due to a small effective mode area4 (0.16 µm2) of the waveguide with cross-section dimension of
320 nm×630 nm. b, SEM picture of the nanotaper tip end at the sample facet. c, Measured insertion loss of
AlGaAsOI waveguides with different lengths showing a linear loss of about 1.4 dB/cm. We measured three waveguides for each length. The waveguides used in the modified cut-back measurement have the same number of bends.
Data 0.08 Fit
0.02 Conversion efficiency
0.00 0.05 0.10 0.15 Pump power (W) Fig. 4 | Nonlinear coefficient estimation by fitting the measured conversion efficiency versus coupled pump power for four-wave mixing in a 3-mm long AlGaAsOI waveguide with cross-section dimension of
320 nm×630 nm. An ultra-high effective nonlinearity of about 660 W-1m-1 was obtained and the derived
5 -17 2 material nonlinearity of Al0.17Ga0.83As is about 2.6×10 W/m , which is similar to typical values previously reported6-8.
External Bandpass Polarization EDFA AlGaAsOI photonic chip cavity laser filter controller Optical spectrum analyzer Fig. 5 | Experimental set-up for frequency comb generation based on the Kerr effect in a micro- resonator. A continuous wave pump laser (Ando AQ4321D), amplified by an erbium-doped fibre amplifier
(EDFA, Amonics AEDFA), was passed through a tuneable band-pass filter (3-dB bandwidth: 16 nm) to minimize amplified spontaneous emission noise. Two lensed fibres were used for fibre-to-chip coupling.
The output spectrum was measured with an optical spectrum analyser (Yokogawa AQ6375). The temperature of the sample substrate was kept at 22.5⁰C to ensure stable coupling. The input and output power were always monitored by a power meter (Hewlett Packard 8153A, not shown) during the experiment.
Power (dBm) -20
-60 1350 1400 1450 1500 1550 1600 1650 1700 1750 1800 Wavelength (nm)
Fig. 6 | Evolution of Kerr frequency comb spectrum when the pump-resonance detuning is decreased
(from the top spectrum to the bottom spectrum). Following primary sideband generation, sub comb lines were generated close to the primary sidebands and finally merged to form a frequency comb with the native line spacing (single-free spectral range), which shows a typical evolution as reported9. The coupled pump power was kept the same (42 mW in this case) during the pump wavelength tuning. a b
20.0 pm 22.4 pm 0.4 0.4 Power (arb.unit) Power (arb.unit) Data 0.2 0.2 Data Fit Fit 0.0 0.0 1549.52 1549.60 1549.68 1551.92 1552.00 1552.08 Wavelength (nm) Wavelength (nm) c d
Power (dBm) -60 -60
1450 1500 1550 1600 1650 1450 1500 1550 1600 1650 Wavelength (nm) Wavelength (nm)
Fig. 7 | Frequency comb generation performances of AlGaAsOI micro-resonators with different aluminium content. a,b, Transmission spectra for resonances for the AlGaAsOI micro-resonator with 15%
(a) and 17% (b) aluminium concentrations. c,d, Measured output spectra when the pump is fine-tuned to a resonance for the micro-resonator with 15% (c) and 17% (d) aluminium concentration. The coupled pump
10 powers are 30 mW and 7 mW in c and d, respectively. As the bandgap of Al0.15Ga0.85As (1.61 eV) is not large enough to suppress two-photon absorption (TPA) efficiently8, optical parametric oscillation (OPO) was not observed in the micro-resonator as shown in c. However, the nonlinear loss can be significantly reduced to a negligible level as the bandgap is increased8. Therefore, a slightly larger bandgap e.g. 1.64 eV
(Al0.17Ga0.83As) results in a significant reduction of TPA and thus enables OPO in the micro-resonator with much lower pump power as shown in d.
-1 nm -1
GVD (ps GVD km 380 nm x 1100 nm -200 380 nm x 1250 nm 380 nm x 1400 nm -300 2000 2500 3000 3500 Wavelength (nm)
Fig. 8 | Dispersion engineering of AlGaAsOI waveguide beyond 2 µm. Anomalous dispersion can be obtained in mid-infrared wavelength range with larger dimension waveguides, which potentially allows mid-infrared frequency comb generation for applications such as molecular spectroscopy11. References
1. Cheng, C. et al. Epitaxial lift-off process for gallium arsenide substrate reuse and flexible electronics.
Nature Commun. 4 1577 (2013).
2. Ottaviano, L., Pu, M., Semenova, E. & Yvind, K. Fabrication of low-loss AlGaAs-on-insulator nano-
waveguide. in preparation.
3. Kobayashi, N., Goto, K., Wakatsuki, T., Komagata, T. & Nakagawa, Y. Improvement of position
accuracy in mask-writing electron beam lithography with a multi-pass writing strategy for reducing
position errors due to resist charging. Proc. SPIE Photomask and Next-Generation Lithography Mask
Technology XV, 7028 70281Y (2008).
4. Afshar V., S. Zhang, W. Q., Ebendorff-Heidepriem, H. & Monro, T. M. Small core optical waveguide
are more nonlinear than expected: experimental confirmation. Opt. Lett. 34 3577-3579 (2009).
5. Agrawal, G. P. Nonlinear Fiber Optics (Academic, 2001)
6. Dolgaleva, K., Ng, W. C., Qian, L. & Aitchison, J. I. Compact highly-nonlinear AlGaAs waveguides
for efficient wavelength conversion. Opt. Express 19 12440-12455 (2011).
7. Lacava, C., Pusino, V., Minzioni, P., Sorel, M. & Critiani, I. Nonlinear properties of AlGaAs
waveguides in continuous wave operation regime. Opt. Express 22 5291-5298 (2014).
8. Wathen, J. J. et al. Efficient continuous-wave four-wave mixing in bandgap-engineered AlGaAs
waveguides. Opt. Lett. 39 3161-3164 (2014).
9. Herr, T. et al. Universal formation dynamics and noise of Kerr-frequency combs in microresonators.
Nature Photon. 6 480-487 (2012).
10. Gupta, M. C. & Ballato, J. The Handbook of Photonics, Second Edition (CRC Press, 2006).
11. Schliesser, A., Picque, N. & Hänsch, T. W. Mid-infrared frequency combs. Nature Photon. 6 440-449